Fluctuations in a melt of flexible. polymers with bonddirected. dipolar monomers

 Matilda Gordon
 3 months ago
 Views:
Transcription
1 Fluctuations in a melt of flexible polymers with bonddirected dipolar monomers by Henry Emmanuel Amuasi Thesis presented in partial fulfilment of the requirements for the degree of MASTER OF SCIENCE at the University of Stellenbosch. Supervisor: Dr. K. MüllerNedeboc October 006
2 DECLARATION I, the undersigned, hereby declare that the wor contained in this thesis is my own original wor and that I have not previously in its entirety or in part submitted it at any university for a degree. 4 th October, SIGNATURE DATE
3 ABSTRACT We employ the Random Phase Approximation (RPA) method to compute the static density and magnetic structure functions of a melt of flexible polymers whose monomers possess bonddirected dipoles which interact with each other. In order to observe the effect of screening of the dipolar interaction on the structure functions we obtain results for cases with and without steric interactions and also for cases with and without DebyeHücel screening of the dipole moments. We show that in all these cases the system exhibits criticality at the same critical Bjerrum length, λ B = 9e 0/ ( 4πρ 0 c l ) where ρ 0 is the monomer concentration, l is the Kuhn length, and c is the ratio of the dipole moment to the length of the bond that constrains it. We also show that in the unscreened cases the dipoledipole structure function is fairly constant diverging at the critical temperature and over all length scales, whereas with screening the dipoledipole structure function exhibits a narrow pea at large length scales and a broad pea at length scales comparable to a few Kuhn lengths. Near the critical temperature the dipoledipole structure function remains finite for all length scales of interest except for a narrow band in the vicinity of the Kuhn length. On the other hand, the density structure function remains finite at all temperatures in both the unscreened and screened cases, but it rather shows a depression in a narrow band in the vicinity of the Kuhn length. OPSOMMING Ons gebrui die metode van die toevalsfasebenadering ( Random Phase Approximation RPA) om die statiese digtheids en magnetiese strutuurfunsies te bereen vir n smelt van hoogsbuigsame polimere, waarvan die monomere dipole langs die verbindings besit wat met meaar in wisselwering tree. Om die effe van afserming op die dipolare wisselwering en die strutuurfunsies te an waarneem, bepaal ons resultate vir die gevalle met en sonder steriese wisselwerings en oo vir gevalle met en sonder die DebyeHücel afserming van die dipoolmomente. Ons wys dat in al hierdie gevalle die stelsel ritiee gedrag by dieselfde ritiee Bjerrumlengte λ B = 9e 0/ ( 4πρ 0 c l ) toon, waar ρ 0 die monomeeronsentrasie, l die Kuhnlengte en c die verhouding van die dipoolmoment tot die lengte van die verbinding is wat dit beper. Ons wys oo dat, in die onafgesermde gevalle, die dipooldipool strutuurfunsie minofmeer onstant is en by die ritiee temperatuur oor alle lengtesale divergeer; inteenstelling, met afserming, toon die dipooldipool strutuurfunsie n nou pie by groot lengtesale en n wye pie by lengtesale wat met n paar Kuhnlengtes vergelybaar is. Naby die ritiee temperatuur bly die dipooldipool strutuurfunsie vir alle lengtesale van belang eindig behalwe vir n nou band in die omgewing van die Kuhnlengte. Andersins bly die digtheidsstrutuurfunsie by alle temperature eindig in beide die onafgesermde en afgesermde gevalle, maar dit toon n afname in nou band in die omgewing van die Kuhnlengte. 3
4 CONTENTS. Introduction Polymer Chains and Melts Polymer Chain Models: Flexibility Long Range Interactions Classification of Polymer solutions The Random Phase Approximation Introducing the Problem: Ferrogels and Polyelectrolytes Ferrogels Polyelectrolytes Layout of the Calculations and Results The Random Phase Approximation Defining the Microstates Collective Coordinates The Mesoscopic Hamiltonian The Transformation Transforming the Potential Energy of Interaction Transforming the Gaussian Chain Energy: the RPA method The Gaussian Chain s BondMatrix Structure Function The Fourier Transform of the Exchange Interaction Analyzing the Collective Hamiltonian RPA with ExcludedVolume Interaction The Transformation The Gaussian Chain s Structure Function The Gaussian Chain s BondVector Structure Function The Collective Hamiltonian Results Asymptotic Behaviour of Gaussian Chain Structure Functions Bondvector density fluctuations Density fluctuations Effect of DebyeHücel Screening Screened Dipolar Interaction Screening without Excluded Volume Interactions
5 Contents.3 Screening and Excluded Volume Interaction Dipoledipole Structure Function for nonzero Screening Length. 69. Structure Functions in the limit of zero Screening Length Conclusion Appendix 78 A. List of symbols B. Inverse of a Special form of a Matrix C. DebyeHücel Screened Dipolar Interaction
6 . INTRODUCTION The purpose of this chapter is to tae the reader through a quic tour of the theory of polymers as found in literature published since the latter half of the last century. The treatise here touches only on those aspects of the literature that are essential to understanding the problem at hand and appreciating the solution presented in the subsequent chapters. The aspects of the literature alluded to in this chapter cover the description of polymers and polymer melts, the mathematical models used to abstract them, and the statistical theories used to investigate them. Next, the chapter devotes a section to describing ferrogels and how they motivate the problem that this thesis is concerned with. The last section gives a general layout of the content of the following chapters.. Polymer Chains and Melts A polymer is a high molecular weight organic compound (a macromolecule), natural or manmade, consisting of many repeating simpler chemical units, or molecules, called monomers. Examples of polymers include polyethylene, polystyrene, and poly(oxyethylene). During its fabrication, a polymer molecule is formed when the energy required to add one more chemical unit (monomer) to the macromolecule is almost independent of the size of the macromolecule. Now consider a closely paced assembly of these polymer molecules. At a sufficiently high temperature, they are in a high state of thermal agitation and form a liquid, called a polymer melt. Alternatively, if these polymers are dissolved in another liquid (called a solvent) then we have a polymer solution. Polymers play a central role in chemical technology and biology. In the latter half of the twentyfirst century it has become possible to offer theories which explain the salient features of polymer melts. Our wor is concerned with the equilibrium properties of a special type of a polymer melt which we describe in Section.6. The geometry of different polymers can be quite diverse. The simplest geometry that a polymer can possess is that of a line. But by means of branching (see Ref. []), polymer molecules can be synthesized with the geometry of stars, combs, treelie structures, or even crosslined networ structures (see Figure.). In our wor we consider polymers with linear geometry called polymer chains. The number of monomers, N, in one polymer chain is often called the index or degree of polymerization of the chain and can be amazingly large. (For example, it is possible to reach N > 0 with polystyrene.)
7 . Introduction 7 LINEAR STAR COMB TREE crosslined Fig..: The various geometrical structures that polymer molecules can have. Quite a number of polymer chain variants are possible. There are two extreme cases: flexible polymer chains and rigid rods (see Figure.). Flexible chains are characterized by being easily bent and being highly coiled. Rigid rods are straight and cannot be easily bent. There exist intermediate cases synonymously nown as semiflexible, semirigid, or stiff polymer chains.
8 . Introduction 8 Flexible polymer Rigid polymer Fig..: Flexible and rigid polymers.. Polymer Chain Models: Flexibility To study the statistical properties of polymer chains, one needs to use a suitable mathematical model to represent a single chain. Many synthetic and biological processable polymers, particularly DNA, are semirigid and have been described in literature [, 3, 4,, 6, 7, 8] using the socalled wormlie polymer chain model. In the wormlie polymer chain model, the polymer chain bacbone is abstracted as an (at least) twicedifferentiable geometric curve R(s) in space. This curve is of finite length L and is parametrized by its arc length s. The tangent vector to this curve at a point s on the curve is constructed as Ṙ(s) = dr(s)/ds and can be shown to be always of unit length (the reason being that the variable parameterizing the curve is the arc length s itself), this is nown as the condition of local inextensibility. The crucial feature of the wormlie polymer chain model, however, is that the Hamiltonian of the polymer chain is a functional H[R(s)] built on the assumption that it costs energy to bend the polymer chain (since it is semirigid). If the tangent vector is constant along the curve then it does not bend. Thus the energy should depend on the derivatives of the unit tangent vector Ṙ(s). We call the the magnitude of R(s) = dṙ(s)/ds the curvature of the curve. The bending energy is also taen to be directly proportional to the temperature T, so that the Boltzmann factor e βh[r(s)] (where β = / B T, B being the Boltzmann constant) is temperature independent: H[R(s)] = ε L 0 ds [ R(s) ]. (.) Hence the partition function for a stiff polymer chain at constant temperature is a functional integral given by Z = D [ Ṙ(s) ] e βh[r(s)] δ 3[( Ṙ(s) ) ], (.) where the integral should be understood as being taen over all chain conformations specified by Ṙ. Note that the delta function in the integrand embodies the
9 . Introduction 9 constraint of local inextensibility. It can be shown (see Ref. []) that at a sufficiently large length scale, that is, at a scale of the order of the persistence length parameter, l p = βε, the wormlie polymer chain behaves as a random wal. One advantage of the wormlie polymer chain model is that by varying the persistence length parameter between the limits l p L and l p L, one may easily scuttle between the extreme limits of flexibility and rigidity respectively. The above model is solvable in principle, but it has been noted [3] that in practice the mathematical difficulties associated with equations governing the states of the wormlie polymer chain model can be formidable. Therefore the wormlie polymer chain model is often considered with auxiliary simplifying assumptions and approximations, such as relaxing the constraint of local inextensibility for instance (see Refs. [3, 7]). Although a fully realistic theory of polymer solutions will involve considerable technical complexity in such matters as the precise flexibility of the molecular linages and the molecular forces, and the nature of the interaction of the molecules with those of the solvent, there remain a core of general functional relationships in, for example the equation of state [9], which can be reduced to problems which are easily posed, but which can only be resolved by fairly powerful mathematical tools. In this dissertation it is hoped to derive the seleton theory in which the dependence of the thermodynamic functions upon the parameters specifying the solution will be demonstrated. For this reason, we avoid the use of the wormlie polymer chain model altogether and employ the discrete version of Edwards Hamiltonian [0], a Hamiltonian which has proven to be a useful and simpler tool in the study of diverse polymer problems [,, 3, 4]. Edwards Hamiltonian is, nevertheless, better suited to highly flexible polymer chains. We defer the full description of this model until Section.3. It suffices for now to say that in this model, the polymer is abstracted as essentially a discrete random wal in space..3 Long Range Interactions Note that in the preceding discussion on single chain models we implicitly limited interactions among monomers to within a few neighbours along the chain. It is these interactions that are responsible for the flexibility (or rigidity) of the chain. In reality, however, monomers distant along the chain do interact if they come close to each other in space (see Figure.3). Following Doi and Edwards [0], we use the term long range interactions to refer to interactions between monomers which are far apart along the chain. This term is used in contrast to short range interactions which represents the interaction among a few neighbouring monomers and is responsible for the local structure of the polymer chain.
10 . Introduction 0 m n Long range interaction Fig..3: Long range interactions (for example the excluded volume interactions) are those interactions that occur between monomers that are far apart along the polymer chain. Note that the term long represents the distance along the chain not the spatial separation An obvious long range interaction is the steric effect: since the monomer has finite volume, other monomers cannot come into its own region. This interaction is nontrivial and reveals itself in the swelling of the polymer; the coil size of a polymer chain with such an interaction is significantly larger than that of the ideal chain which has no such interaction. This effect is nown as the excluded volume effect []. The type of polymer chains which we deal with in this dissertation consists of monomers which also possess dipole moments. Consequently, another long range interaction appears: the dipolar interactions. This interaction is fully described in Section.3. In polymer melts, or solutions, interactions also exist between different polymers. These interpolymer interactions are comprised of those interactions (also classified as long range interactions) between monomers on different polymer chains. In the second chapter of this dissertation we investigate the flexible chain model with such dipolar interactions included but without the excluded volume effect, and in the third chapter we include the excluded volume interactions..4 Classification of Polymer solutions A polymer melt may most generally be described as a system of a large number, say N p, of polymer chains assembled together in a finite region of space of volume. If this space is also mediated by a liquid (called a solvent), then we have a polymer solution. Naturally such systems, because of the large number of particles (the monomers) constituting its polymer chains, lend themselves to useful study by means of equilibrium statistical methods. Edwards [9, 0] in 966, put forward a simple description of such systems, classifying them
11 . Introduction into three broad regimes determined by the parameters of the solution: N the number of monomers per polymer chain (also called the index of polymerization), N p the number of polymer chains, l the effective length of a polymer bond, v the excluded volume per monomer which may also be viewed as the effective volume per monomer (the definition of v is given in Section 3.4), and the total volume. The regimes Edwards identified are the (a) dilute, (b) semidilute, and (c) concentrated regimes of polymer solutions. A dilute solution is defined as one of sufficiently low concentration that the polymer chains are separated from one another; each polymer on the average occupying a spherical region of radius R g (called the radius of gyration). Now if we assume each polymer chain to be a random wal of N steps, then R g Nl and this regime may be described by the following relation: ( N l ) 3 /Np. (.3) A dilute solution is characterized by a small mean density (or concentration) of monomers NN p / and by large spatial fluctuations localized over regions of size comparable to that of a polymer chain. These fluctuations are illustrated in Figure.4. In such solutions the polymer polymer interaction is very small. As the concentration of polymers is increased (that is as N p is increased) we enter the semidilute solution regime in which ( N l ) 3 /Np. (.4) In this regime, though the mean concentration of polymers, N p /, (or their volume fraction NN p v/) is still small, the polymer chains are long enough (N l large) to cause strong overlapping among themselves. A semidilute solution is characterized by a mean density with large and strongly correlated spatial fluctuations in the local monomer concentration as illustrated in Figure.4. A concentrated solution is one of sufficiently high concentration that /N N p v. (.) In this case, the mean concentration of monomers becomes large, and the fluctuations become small compared to the mean concentration of monomers (as illustrated in Figure.4). Hence this regime becomes amenable to treatment by a mean field theory including small spatial fluctuations (up to quadratic order approximation). This mean field theory is variously nown as the Random Phase Approximation (RPA) or the Gaussian Approximation. Such is the nature of our concerns in this dissertation.
12 . Introduction c(x) c(x) c(x) c c c x x x (a) dilute (b) semidilute (c) concentrated Fig..4: Three concentration regimes of polymer solutions. c(x) denotes the concentration profile along the dotdashed lines.. The Random Phase Approximation It was de Gennes [6] who pointed out that the meanfield theory is rather good for high molecular mass (large N) polymer melts, in contrast to low molecular mass polymer melts, for which the meanfield theory breas down close to the critical point. His argument was based on the Ginzburg criterion [4, 6, 7, 8] which states that the meanfield approach is quantitatively correct if the fluctuations of the monomer concentration are small compared to the mean concentration near the critical point. He found that for large N the meanfield theory breas down very close to the critical temperature T c, that is for (T T c )/T c /N. Thus in the limit of N, the meanfield theory is correct in the whole region around the critical point. The random phase approximation is a term that has been used to describe various approaches to calculating the fluctuations in the mean field theory of polymers. Some authors [4] derive the theory by applying a special form of the fluctuationdissipation theorem [7] in which the fluctuations of the local concentration field of monomers, δρ(r) = ρ(r) ρ 0 (or some other chosen order parameter such as the local magnetization field u(r)), may be written using two different expressions. In the first relation, δρ(r) is written as being modified in response to a spatiallyvarying external field, h(r), plus a spatiallyvarying molecular field, w m (r), written in the mean field approximation and representing the mean interaction of all the other monomers in the system with any single monomer: δρ(r) = d 3 r χ 0 (r, r )[h(r) + w m (r)], (.6)
13 . Introduction 3 where w m (r) = d 3 r w(r, r ) ρ(r) = d 3 r w(r, r ) δρ(r) + ρ 0, (.7) and w(r, r ) represents the interaction potential between the monomers. The fluctuationdissipation theorem then states that the response function, χ 0 (r, r ), of such a relation is directly proportional to the densitydensity pair correlation function, δρ(r)δρ(r ) 0 of noninteracting polymers, which can be readily computed. In the second relation, δρ(r) is written as being modified in response to the spatiallyvarying external field, h(r) alone: δρ(r) = d 3 r χ(r, r ) h(r), (.8) and hence the response function, χ(r, r ), in such a relation is directly proportional the true densitydensity pair correlation function, δρ(r)δρ(r ), of the melt. Thus these two equations ((.6) and (.8)) are equated and the resulting integral equation is solved selfconsistently for the true response function (or densitydensity correlation function) of the melt. In our wor, however, we do not employ this method. Our approach to the RPA instead employs a Gaussian approximation in which an attempt is made to obtain a Hamiltonian written as a functional of the order parameter ρ(r) the local density field (or u(r) the local magnetization field). Technically, one is able to do so successfully only up to quadratic order in these parameters. Vilgis, Weyersberg, Jarova, and Brereton [, ] also employ this method. However, unlie Vilgis and Jarova [3], we do not approximate the dipolar interaction by an approximate shortrange function, but we apply the exact unscreened dipolar interaction [9] (see equation (.3)) between pairs of dipoles. We later also apply DebyeHücel [7] screening to the dipolar interaction. One surprising result of our calculations for the density fluctuations for the unscreened case is that we do not observe any of the usual indications of microdomain structure as put forward by Leibler [0], that is, the density structure function obtained does not show any peas or singularities anywhere within the domain of length scales comparable to the length scale of the size of a polymer (the radius of gyration R g ). Neither does the density structure function indicate a phase transition at any temperature. However, our investigations into the magnetization fluctuations made us to rediscover the fluctuationinduced longrange orientational correlations mentioned by Vilgis, Weyersberg and Brereton []. These correlations appear to increase over all length scales as the temperature is lowered towards a certain critical temperature where the isotropic phase breas down. This temperature also signals the breadown of the Gaussian approximation.
14 . Introduction 4.6 Introducing the Problem: Ferrogels and Polyelectrolytes In this wor, we consider in particular the fluctuations in a concentrated polymer melt of fixed volume at a constant temperature, and whose polymer chains are made up of dipolar monomers whose dipole moments are constrained to lie along the polymer chain bacbone; all dipoles on a polymer having the same sense of direction along the chain. The description of such a polymer is illustrated in Figure.3 on page. Thus the monomers interact with each other via the dipolar potential energy of interaction. We investigate not only fluctuations of the local monomer concentration field (or density order parameter), but also the fluctuations of the local dipole moment vector field (or magnetization order parameter). The reader may wonder why we investigate a melt of this peculiar type of polymer. There are at least two reasons. One reason is that this type of polymer melt is a very simplified model that has been proposed in recent literature [3] as a first attempt to understand the thermodynamic properties of magnetic field sensitive polymer gels called ferrogels. The other reason is because this model can be understood as a limit of certain polyampholytes [], which are polymers in solution with alternating charges distributed along their bacbone. Recently both ferrogels and polyelectrolytes have been of considerable research interest because of their various applications in soft matter physics..6. Ferrogels A ferrogel is a chemically crosslined polymer networ swollen by (or dissolved in) a ferrofluid [, 3, 4, ]. A ferrofluid, or a magnetic fluid, is a colloidal dispersion of monodomain magnetic particles. Their typical size is about 0 nm and they have superparamagnetic behaviour. In the ferrogel, the finely distributed magnetic particles are located in the swelling liquid and attached to the crosslined networ chains by adhesive forces. These solid particles of colloidal size are the elementary carriers of a magnetic moment. In the absence of an applied magnetic field the moments are randomly oriented, and thus the gel has no net magnetization. As soon as an external field is applied, the magnetic moments tend to align with the field to produce a bul magnetic moment. With ordinary field strengths, the tendency of the dipole moments to align with the applied field is partially overcome by thermal agitation, such as the molecules of a paramagnetic gas. As the strength of the magnetic field increases, all the particles eventually align their moments along the direction of the field, and as a result, the magnetization saturates. If the field is turned off, the magnetic dipole Superparamagnetism occurs when the material is composed of very small crystallites ( 0 nm). In this case, even though the temperature is below the Curie or Neel temperature and the thermal energy is not sufficient to overcome the coupling forces between neighboring atoms, the thermal energy is sufficient to change the direction of magnetization of the entire crystallite. The resulting fluctuations in the direction of magnetization cause the magnetic field to average to zero. The material behaves in a manner similar to paramagnetism, except that instead of each individual atom being independently influenced by an external magnetic field, the magnetic moment of the entire crystallite tends to align with the magnetic field.
15 . Introduction moments quicly randomize and thus the bul magnetization is again reduced to zero. In a zero magnetic field a ferrogel presents a mechanical behaviour very close to that of a swollen networ filled with nonmagnetic colloidal particles. Some ferrogels belong to a larger class of adaptive (smart, intelligent) materials called polymer gels [6]. These materials can actuate, or alter their properties in response to a changing environment. Among them mechanical actuators have been the subject of much investigation in recent years. They undergo a controllable change of shape due to some external physical effects and can convert energy (electrical, thermal, chemical) directly to mechanical energy. This can be used to do wor against load. Certain polymer gels represent one class of actuators that have the unique ability to change elastic and swelling properties in a reversible manner. These wet and soft materials offer lifelie capabilities for the future direction of technological development. Volume phase transition in response to infinitesimal change of external stimuli lie ph, temperature, solvent composition, electric field, and light has been observed in various gels. Their application in devices such as actuators, controlled delivery systems, sensors, separators and artificial muscles has been suggested and are in progress. Attempts at developing stimuliresponsive gels for technological purposes are complicated by the fact that structural changes, lie shape and swelling degree changes that occur, are inetically restricted by the collective diffusion of chains and the friction between the polymer networ and the swelling agent. This disadvantage often hinders the effort of designing optimal gels for different applications. In order to accelerate the response of an adaptive gel to stimuli, the use of magnetic field sensitive gels as a new type of actuator has been developed [4]. Magnetic field sensitive gels, or as we call them ferrogels, are typical representatives of smart materials. Naturally, a theory for ferrogels is very difficult and suffers from many different length scales. The development of a single theory that taes into account all the aspects of ferrogels seems to be too difficult. Therefore we aim here for a much simpler model, which might not be capable of describing the experimental results in detail, but give first hints of methods and solutions. Following Vilgis and Jarova [3] we assume that the magnetic moments are placed along the contour of the chains. In the light of the foregoing discussion, this assumption seems to be rather unrealistic. Nevertheless it enables some calculations to be performed and the prediction of results for polymer melts that involve magnetic interactions. Therefore we assume that each monomer carries a dipole moment whose main axis points in the direction of the tangent vector. This assumption is made only to ease calculations. The magnetic particles couple somehow to the polymer chains but no one so far has resolved this mechanism. We also neglect the crosslins between polymer chains thus releasing the chains to move freely with respect to each other. This situation is completely changed when the chains are crossedlined to each other to form a networ. The crosslins restrict the chain motion significantly and the phase depends naturally on the crosslining state. (See Ref. [3] for a treatment of both the uncrosslined case and the crosslins using quenched variables.)
16 . Introduction 6 Our point of departure from the wor of Vilgis and Jarova [3] is that we utilize the exact expression for the dipolar interaction between a pair of dipoles p and p separated by a vector r: U(p, p, r) = λ B β ( ) p p 3 (ˆr p ) (ˆr p ) r 3, (.9) instead of the shortranged isotropic function given as an approximation to the expression above U (p, p, r) = J 0 δ(r)p p, (.0) where J 0 is a constant. Our reasons for investigating the true form of the dipolar function are that, as Zhang and Widom [7, 8] have pointed out, two characteristics of dipoles lead to unusual difficulties in analyzing these systems: long range and anisotropy. The r 3 falloff leads to conditional convergence of the local field due to a distribution of dipoles at remote locations. The anisotropy in the numerator of equation (.9) leads to frustration in aligning favourably with nearby dipoles..6. Polyelectrolytes Polyelectrolytes may widely be defined as highly charged macromolecules or aggregates formed in aqueous solution by dissociation of charged units of these macromolecules. Many important biological macromolecules are polyelectrolytes. The most important example is DNA and RNA molecules, which dissociate in solution forming a strongly negatively charged polyion surrounded by atmosphere of small mobile counterions. Protein molecules in solution usually contain polar groups of the both signs. There exists also many synthetical polyelectrolytes with important technological applications. By a process nown as adsorption mobile charges from the bathing solution and fixed charges along the polyelectrolyte can combine, leading to the emergence of higher multipoles along the polyelectrolyte chain, the first one being a dipole stemming from the association of a negative fixed charge on the polyelectrolyte and a specifically adsorbed mobile charge from the bathing solution. Muthuumar [] and Podgorni [7] have wored on dipolar flexible and dipolar semiflexible single chains respectively. Muthuumar, by using the Edwards Hamiltonian, discovered the formation of localized aggregated structures along the chain that dominate the statistical behaviour of the flexible polyelectrolyte chain, while Podgorni, by means of the wormlie chain model, discovered how screening of the dipolar interaction modifies the persistence length of an otherwise bare neutral polymer..7 Layout of the Calculations and Results The content of the following chapters is structured along the following lines: in Chapter we aim to introduce the Random Phase Approximation (RPA) by
17 . Introduction 7 calculating the Hamiltonian (or the partition function) and the dipoledipole structure function for a melt of unscreened dipolar polymers whose monomers do not have any volume, and hence they do not exclude each other. In Chapter 3 we perform RPA computations again for the same melt, but this time with the excluded volume interaction included between its monomers. We obtain results for the Hamiltonian in terms of monomer and bond vector concentrations. Next, Chapter 4 presents and analyzes the results of Chapter 3. It shows some plots of the dipoledipole structure function and of the density structure function and proposes that the reason for their shape is due to the longrange character of the unscreened dipole potential. Then Chapter gives the RPA results for the case of DebyeHücelscreened dipolar interactions. Lastly Chapter 6 concludes by highlighting all the results obtained in this dissertation and also offers possible further directions for future investigation.
18 . THE RANDOM PHASE APPROXIMATION Our quest is to obtain, in as closed form as possible, the partition function of a melt or solution of polymer chains with dipole moments directed along the chains and which is in thermal equilibrium with its surroundings at a constant temperature. This thermodynamic system offers itself to simple mathematical treatment while capturing most of the essential features of polymer solutions that an experimentalist may encounter in practice. The traditional recipe to obtaining the partition function is as follows:. Identify, or define, the different microstate variables of the system. (We have some freedom in fulfilling this requirement. As we will see later, the particular set of microstate variables one chooses depends on the observer of the system.). Construct the Hamiltonian of the system. The Hamiltonian may be seen to be a function over microstatespace, assigning to each state a scalar value nown as the energy or cost of the system being in that state. The Hamiltonian is also parametrized by the macrostate variables (such as the temperature, volume, etc.) of the system. These macrostate variables represent the constraints imposed on the system by its environment. 3. Determine the probability associated with the energy of each state. This probability is nown as the Boltzmann factor of the state. 4. Sum the Boltzmann factors over all the states to obtain the partition function. Once the partition function has been obtained, various equilibrium statistical properties of the system can be extracted from it by applying their corresponding operators on the partition function. In favour of the simplicity of the mathematical treatment we shall assume in this chapter that the monomers of our polymer chains do not possess any volume and hence do not exclude each other in space. In the next chapter we shall treat also the excluded volume interactions.. Defining the Microstates Upon first consideration, the different microstates of our system depend on the different conformations in space that each polymer can tae. It is not
19 . The Random Phase Approximation 9 difficult to describe the different conformations of a single polymer chain: we simply use a sequence of the threedimensional position vectors of the monomers along the chain, for example, for a polymer with N + monomers we may use {r n } n=0,...,n or {r 0,b n } n=,...,n where r n denotes the position vector of the nth monomer along the polymer chain and b n = r n r n is the bond vector directed from r n to r n. For a melt of polymer chains we need, in addition, to label each polymer. Let us use the index α to label each polymer. Thus supposing we have in our melt N p polymers, then a state of our system is sufficiently identified by the sequence {r α n} α=,...,np n=0,...,n α or {r α 0,b α n} α=,...,np n=,...,n α. We will assume for simplicity that all polymers in the melt have the same number, N, of monomers. It is common practice in polymer physics to define the socalled mesoscopic Hamiltonian, H({r n }), over conformations of the polymer chain as described as above. It turns out however that for the problem at hand we need a different set of variables to describe the states for our system. Remembering that our system has dipoles attached to the monomers, we thus anticipate that at low temperatures the dipolar interactions between the monomers in the melt win over their thermal agitations, and hence will give rise to microdomain structure, a phase in which longrange order of the dipoles appears. Consequently, spatial fluctuations in the local magnetization field, m(r) (and possibly the local density field ρ(r)), become significant on a scale which is large compared with the typical bondlength of the polymer chains. The fluctuations in density may be characterized by a densitydensity correlation function [0, 4]: S(r r ) = β ρ(r ) ρ(r ), (.) where β = / B T, T being the temperature, and B is the Boltzmann constant. Here... denotes the thermal average. The Fourier transform, S(), of S(r) can be studied by means of elastic radiation scattering experiments: light, Xray, or neutron scattering. (Here denotes the scattering wavevector, which may be roughly viewed as the reciprocal distance between planes of monomers in the melt.) In such experiments, the intensity, or more precisely, the differential crosssection [7], of radiation detected at a given is directly proportional to S(). The scattering power, S(), can be calculated with the Random Phase Approximation (RPA) method, which will be this chapter s main focus. So we imagine a beam of neutrons incident on our melt of polymers with dipoles directed along the polymer bonds. These neutrons (which possess intrinsic dipole moments) will interact with, and hence be scattered off, the scattering units of the system, which we will assume to be only the dipolar monomers directed along the polymer chains. Hence the camera, or detector, recording these scattering events will see only the spatial distribution, or field of dipolar monomers of the system: the observer is, to some extent, oblivious to the particular conformations of the polymer chains that presented a particular spatial distribution of dipolar monomers (see Figure.). In fact, there may be many different conformations of the polymer chains (or microstates of the system) that conform to the same dipole distribution. Our tas therefore, is to collect all polymer conformations corresponding
20 . The Random Phase Approximation 0 (a) (b) Fig..: (a) The medium being investigated as perceived in the mind of the observer. (b) The same medium being investigated, but as seen by the detector of the scattering experiment: the detector is oblivious to the particular conformation that presented this dipole distribution. to a particular dipole distribution and label them all as one microstate which we will call the collective microstate. This tas will amount to transforming the mesoscopic Hamiltonian, defined over polymer conformations, into a new Hamiltonian defined instead over dipole distributions. We hereby introduce the socalled collective coordinates so that whereas microstate coordinates label the microstates of the mesoscopic Hamiltonian, collective coordinates label the collective microstates of the collective Hamiltonian.. Collective Coordinates We introduce the following definitions for collective coordinates []:. The monomer density (or concentration) collective coordinate: ρ(r) δ (3) (r r α n), (.) and. the bondvector density collective coordinate: u(r) δ (3) (r r α n)b α n, (.3) where we have set b α 0 = 0 for all α.
21 . The Random Phase Approximation These new fields, ρ(r) and u(r), may each be considered to be a superposition of a large number of planewavelie fluctuations of different wavelengths, so that these new fields can each be rewritten as ρ(r) = ρ e i r = (π) 3 d 3 ρ e i r, u(r) = u e i r = (π) 3 d 3 u e i r, (.) where the amplitudes ρ and u are, respectively, the Fourier transforms for. the density collective coordinate: and for ρ F [ ρ(r) ] d 3 r = ei r ρ(r) d 3 r = ei r δ (3) (r r α n) = e i rα n, (.6). the bondvector density collective coordinate: u F [ u(r) ] d 3 r = ei r u(r) d 3 r = ei r δ (3) (r r α n)b α n = e i rα n b α n. (.7) The amplitudes, ρ and u, represent the spatial fluctuations of ρ(r) and u(r) on a scale given by. It is clear from their representations that ρ and u are, in general, complex except for ρ 0 and u 0, which are real. Moreover notice that not all ρ and u are independent of each other since ρ  = ρ and u  = u. (.8) Notice that in equation (.) we presented, on purpose, two formally distinct ways of representing the fields u(r) and ρ(r): the series and the integral representations. We point out here that each representation furnishes its own expression for the threedimensional Dirac delta function, as shown in the following equation: δ (3)`r r = X Z e i (r r ) = (π) 3 d 3 e i (r r ). (.4) In the rest of this document, we chose to use the more succinct series representation.
22 . The Random Phase Approximation In the rest of this document, the reader will encounter such abbreviated notation as > 0, 0, or 0 : > 0 refers to the region in threedimensional space described by { x, y, z > 0} (the upper halfspace) where x, y, and z are the x, y, zcomponents of ; 0 is > 0 and = 0; and 0 means all of space excluding the origin. As we shall see later, there is an advantage to woring in space, namely, it eventually enables us to compute the partition function, after a suitable approximation, by performing a Gaussian integral with an already diagonalized quadratic form over the phase amplitudes..3 The Mesoscopic Hamiltonian The mesoscopic Hamiltonian gives the energy of polymer chains modeled by Gaussian chains whose bonds (such as b α n) follow the threedimensional Gaussian distribution: ( ) 3 ] 3 p(b α n) = exp [ 3(bα n) πl l. (.9) where the constant l is called the Kuhn length or the effective bond length of the polymer (and not the actual bond length, for reasons soon to be given). So (b α n) = l. (.0) The conformational distribution function of a melt of Gaussian chains is therefore P({b α n}) = ( ) 3 ] 3 exp [ 3(bα n) πl l ( ) [ 3 3NNp = πl exp  ] (.) 3(b α n) l The Gaussian chain does not describe correctly the local structure of the polymer because the Gaussian chain assumes statistical independence of adjacent bonds, which is generally not true for most polymers because of shortrange interactions between neighbouring monomers along the chain. But the Gaussian chain does correctly describe the structure on a large enough scale (i.e., the mesoscopic scale) because for most types of polymers (and polymer models) bondtobond correlation decreases rapidly (roughly exponentially) with increasing separation between the bonds along the polymer. Hence any type of polymer chain may be subdivided into, say, N submolecules each consisting of, say, λ bonds, so that b α n is actually the endtoend vector of one of these submolecules, and l is the rootmeansquare length of one of these submolecules, hence its name: effective bond length. The parameter, λ, can be taen to be large enough so that the vectors b α n become independent of each other. The advantage of the Gaussian
23 . The Random Phase Approximation 3 chain is that it is mathematically much easier to handle than other models. The Gaussian chain is also referred to as the ideal chain. The Gaussian chain is often represented by a mechanical model in which (N + ) monomers are considered to be interconnected by harmonic springs whose total potential energy is H 0 ({b n }) = 3 β l (b n ). (.) Thus the spring constant of each bond is 3/βl which is temperaturedependent. Using the above expression for our Hamiltonian of a melt of polymers, we see that at equilibrium, the Boltzmann factor, exp ( β H 0 ({b α n})) for a melt of polymers is exactly the same as the exponential factor in equation (.). While the Gaussian chain effectively describes polymer chains with interactions existing between neighbouring monomers along the same polymer chain, it fails to account for interactions that may exist between monomers separated far apart on the polymer chain, such as dipolar interactions (since the monomers are assumed to possess dipole moments) and excluded volume interactions. Therefore such interactions should be added to the mesoscopic Hamiltonian by hand. In this chapter we shall treat only the dipolar interactions, then in the following chapter we shall also include the excluded volume interaction. The interaction energy between two dipoles with dipole moments, say, p and p separated by a separation vector, say, r directed from p to p is U(p, p, r) = λ B βe 0 ( n p p 3 (ˆr p ) (ˆr p ) r 3 ), (.3) where ˆr = r/ r, λ B is the Bjerrum length [7], and e 0 is the electron charge. Note that implicitly the Bjerrum length is directly proportional to β (see Appendix A) so that U(p, p, r) is temperatureindependent, but the Boltzmann factor exp ( β U) is temperaturedependent. Figure. illustrates the essential features of the dipolar interaction. The total dipolar energy of interaction in a melt of polymers includes interactions between monomers on different polymer chains, and is therefore U({p α n, r α n}) = λ B βe 0 = λ B βe 0 α, β n>m p α n p β m 3 (ˆr α n m β p α n r β m r α n 3 p α n 3 ˆrα n m β ˆrα n m β r β m r α n 3 p β m, α, β n>m ) (ˆr α β n m p β m ) (.4) where ˆr α n m β = ( r β m rn) α / r β m r α n. If furthermore the dipoles are constrained to align themselves with the bonds along the polymer chain to which they belong, that is, p α n = c b α n (.)
24 . The Random Phase Approximation 4 S N Energetically favourable configurations (a) Energetically unfavourable configurations (b) Fig..: (a) The field in a vertical plane through a dipole depicted as a sphere; each field line in the diagram shows the direction that another dipole is most liely to point at if placed at a point along that field line. (b) Energetically favourable and energetically unfavourable configurations of a pair of dipoles. where c is a dimensionful constant, then U({r α n}) = λ B C β b α n 3 ˆrα n m β ˆrα n m β r β m r α n 3 b β m, (.6) α, β n>m where C = c /e 0 (.7)
25 . The Random Phase Approximation r α 0 r α n b α r α b α n b α n r α n b α r α n r α b α n 0 = 0 polymer α D (b α n) E 0 = l Fig..3: A diagram showing a section of a typical polymer chain of our model with dipoles (represented by the arrows) directed along the chain. Hence, finally, our mesoscopic Hamiltonian is H({r α n}) = 3 β l (b α n) + λ B C β b α n 3 ˆrα n m β ˆrα n m β r β m r α n 3 b β m, (.8) α, β n>m and we may now proceed with the transformation of this Hamiltonian into another Hamiltonian defined over collective variables..4 The Transformation We point out here that, in principle, when we consider the microstates of a physical system we should tae into account not only the positions of the particles in the system but also their momenta. This consideration, however, leads to an (uninteresting) additional term in the Hamiltonian, namely the inetic energy. Hence the full partition function, Z, is an integral over momentumspace and positionspace (collectively called phasespace). Moreover, after integrating over momentumspace alone, the inetic energy term in the Hamiltonian only leads to an uninteresting dimensionful factor, Z m, in the full partition function. The remaining factor is the conformational partition function, Z c, since it is an integral over positionspace variables alone, that is, over conformations in positionspace. Thus Z = Z m Z c. (.9) The dimensions of Z m are / [ L d] where [L] denotes the dimensions of length and d is the number of degrees of freedom of the system Z describes. Since Z is dimensionless, then Z c has dimensions of [ L d]. For our system of a melt of
26 . The Random Phase Approximation 6 polymers we have Z c = Db e β H0({rα n }) e β U({rα n }) (.0) where Db is a measure which must have the same dimensions as Z c. The integrand of equation (.0) may be considered to be a probability density function of random variables {r α n}. Then our crossingover to collective variables will amount to finding the probability density function of a new random variable, such as {u }, which is itself a function of {r α n}. The standard technique to finding this new probability density function is to first treat {u } and {r α n} as independent variables. Next, introduce as a new factor into the integrand of equation (.0), the Dirac delta containing the functional dependency between {u } and {r α n}. Finally, integrate over {r α n}. As a result, the conformational partition function transforms into an integral over the {u }. This technique is summed up in the following equation: we need to find a H 0 ({u }) and U({u }) such that the following equation holds Z c = Du e β H0({u}) e β U({u }) = Du Db 0δ ( ) u e i rα n b α n e β H0({rα n }) e β U({rα n }).. Transforming the Potential Energy of Interaction (.) Incidentally it is much easier to transform U({r α n}): in fact, as we now show, U({r α n}) may simply be rewritten in terms of {u }. First, we find that U({r α n}), as given in equation (.6), may be written as U({r α n}) = b α n J ( r α n r β m) b β m ( δ α β δ n m ), (.) α, β n, m the prefactor of having been included to ensure summation over distinct pairs of monomers, while the trailing factor of ( δ α β δ n m ) has been included to ensure summation over distinct monomers. We label J (r) as an exchange interaction and it has the form J (r) = λ BC β 3ˆrˆr r 3. (.3) To avoid having to carry these factors around all the time, we simply define a slightly modified exchange interaction, J(r), as J(r) λ BC β 3ˆrˆr r 3 ( δ r, 0 ). (.4)
27 . The Random Phase Approximation 7 Now let J be the Fourier transform of J(r), that is, J(r) = J e i r. (.) Therefore equation (.) may be rewritten as U({r α n}) = [ ] b α n J e i (rα n rβ m) b β m α, β n, m = ] ] [e i rα n b α n J [e i rβ m b β m = α, β n, m u  J u U({u }). (.6) We shall postpone the calculation of J till after the next section..6 Transforming the Gaussian Chain Energy: the RPA method Now that we have successfully transformed the potential energy of interaction, all that remains is to transform the Gaussian chain energy: H 0 ( {b α n } ) = a β (b α n) (.7) where a = 3 l. We want to find a new Hamiltonian, H 0 ({u }), defined over states determined by the sets {u }. Referring to equation (.) we see that this new Hamiltonian is given by as e β H0({u}) = Db ( ) δ ()(3) u e i rα n b α n >0 ( ) δ (3) u 0 b α n e β H0({bα n }), (.3) The Dirac delta, δ () (z) (where z = x+iy ; x, y R), over the complexplane is defined, Let = x+iy and so that δ () (z) = δ(x)δ(y) = Z ZZ d dx d y. Then Z Z dx eix x dy eiy y. (.8) π π xx + yy = z + z (.9) δ () (z) = Z d π ei( z+z ). (.30)
EXAM I COURSE TFY4310 MOLECULAR BIOPHYSICS December Suggested resolution
page 1 of 7 EXAM I COURSE TFY4310 MOLECULAR BIOPHYSICS December 2013 Suggested resolution Exercise 1. [total: 25 p] a) [t: 5 p] Describe the bonding [1.5 p] and the molecular orbitals [1.5 p] of the ethylene
More informationPHASE TRANSITIONS IN SOFT MATTER SYSTEMS
OUTLINE: Topic D. PHASE TRANSITIONS IN SOFT MATTER SYSTEMS Definition of a phase Classification of phase transitions Thermodynamics of mixing (gases, polymers, etc.) Meanfield approaches in the spirit
More informationStatistical Thermodynamics Exercise 11 HS Exercise 11
Exercise 11 Release: 412215 online Return: 1112215 your assistant Discussion: 1512215 your tutorial room Macromolecules (or polymers) are large molecules consisting of smaller subunits (referred to as
More informationSwelling and Collapse of Single Polymer Molecules and Gels.
Swelling and Collapse of Single Polymer Molecules and Gels. CoilGlobule Transition in Single Polymer Molecules. the coilglobule transition If polymer chains are not ideal, interactions of nonneighboring
More information3 Biopolymers Uncorrelated chains  Freely jointed chain model
3.4 Entropy When we talk about biopolymers, it is important to realize that the free energy of a biopolymer in thermal equilibrium is not constant. Unlike solids, biopolymers are characterized through
More informationPolymer dynamics. Course M6 Lecture 5 26/1/2004 (JAE) 5.1 Introduction. Diffusion of polymers in melts and dilute solution.
Course M6 Lecture 5 6//004 Polymer dynamics Diffusion of polymers in melts and dilute solution Dr James Elliott 5. Introduction So far, we have considered the static configurations and morphologies of
More informationEntanglements. M < M e. M > M e. Rouse. Zeroshear viscosity vs. M (note change of slope) Edwards degennes Doi. Berry + Fox, slope 3.4.
Entanglements Zeroshear viscosity vs. M (note change of slope) M < M e Rouse slope 3.4 M > M e Edwards degennes Doi slope 1 Berry + Fox, 1968 Question: Which factors affect the Me: T, P, M, flexibility,
More informationPolymer solutions and melts
Course M6 Lecture 9//004 (JAE) Course M6 Lecture 9//004 Polymer solutions and melts Scattering methods Effects of excluded volume and solvents Dr James Elliott Online teaching material reminder Overheads
More informationPolymer Dynamics and Rheology
Polymer Dynamics and Rheology 1 Polymer Dynamics and Rheology Brownian motion Harmonic Oscillator Damped harmonic oscillator Elastic dumbbell model Boltzmann superposition principle Rubber elasticity and
More informationColloidal Suspension Rheology Chapter 1 Study Questions
Colloidal Suspension Rheology Chapter 1 Study Questions 1. What forces act on a single colloidal particle suspended in a flowing fluid? Discuss the dependence of these forces on particle radius. 2. What
More informationRudiments of Polymer Physics
Rudiments of Polymer Physics Justin Bois California Institute of Technology Student of Niles Pierce and ZhenGang Wang 4 July, Rudiments of Polymer Physics 1 1 Introduction A polymer is a chain of several
More informationPolymers. Hevea brasiilensis
Polymers Long string like molecules give rise to universal properties in dynamics as well as in structure properties of importance when dealing with: Pure polymers and polymer solutions & mixtures Composites
More informationOlle Inganäs: Polymers structure and dynamics. Polymer physics
Polymer physics Polymers are macromolecules formed by many identical monomers, connected through covalent bonds, to make a linear chain of mers a polymer. The length of the chain specifies the weight of
More informationENAS 606 : Polymer Physics
ENAS 606 : Polymer Physics Professor Description Course Topics TA Prerequisite Class Office Hours Chinedum Osuji 302 Mason Lab, 4324357, chinedum.osuji@yale.edu This course covers the static and dynamic
More informationAn Introduction to namic Light Scattering by Macromole cules
An Introduction to namic Light Scattering by Macromole cules Kenneth S. Schmitz Department of Chemistry University of MissouriKansas Kansas City, Missouri City ACADEMIC PRESS, INC. Harcourt Brace Jovanovich,
More informationBrownian Motion and Langevin Equations
1 Brownian Motion and Langevin Equations 1.1 Langevin Equation and the Fluctuation Dissipation Theorem The theory of Brownian motion is perhaps the simplest approximate way to treat the dynamics of nonequilibrium
More informationColloidal Particles at Liquid Interfaces: An Introduction
1 Colloidal Particles at Liquid Interfaces: An Introduction Bernard P. Binks and Tommy S. Horozov Surfactant and Colloid Group, Department of Chemistry, University of Hull, Hull, HU6 7RX, UK 1.1 Some Basic
More informationRoland R. Netz MaxPlanck Institute for Colloids and Interfaces, Potsdam, Germany
282 2 Electrochemical Double Layers 2.7 Polyelectrolytes in Solution and at Surfaces Roland R. Netz MaxPlanck Institute for Colloids and Interfaces, Potsdam, Germany David Andelman School of Physics and
More informationThe finegrained Gibbs entropy
Chapter 12 The finegrained Gibbs entropy 12.1 Introduction and definition The standard counterpart of thermodynamic entropy within Gibbsian SM is the socalled finegrained entropy, or Gibbs entropy. It
More informationINTERMOLECULAR AND SURFACE FORCES
INTERMOLECULAR AND SURFACE FORCES SECOND EDITION JACOB N. ISRAELACHVILI Department of Chemical & Nuclear Engineering and Materials Department University of California, Santa Barbara California, USA ACADEMIC
More informationLight scattering Small and large particles
Scattering by macromolecules E B Incident light Scattered Light particle Oscillating E field from light makes electronic cloud oscillate surrounding the particle Intensity: I E Accelerating charges means
More information3. General properties of phase transitions and the Landau theory
3. General properties of phase transitions and the Landau theory In this Section we review the general properties and the terminology used to characterise phase transitions, which you will have already
More informationParticle Characterization Laboratories, Inc.
Analytical services Particle size analysis Dynamic Light Scattering Static Light Scattering Sedimentation Diffraction Zeta Potential Analysis Single Point Titration Isoelectric point determination Aqueous
More information2.1 Traditional and modern applications of polymers. Soft and light materials good heat and electrical insulators
. Polymers.1. Traditional and modern applications.. From chemistry to statistical description.3. Polymer solutions and polymer blends.4. Amorphous polymers.5. The glass transition.6. Crystalline polymers.7.
More informationAmorphous Polymers: Polymer Conformation Laboratory 1: Module 1
D E P A R T M E N T O F M A T E R I A L S S C I E N C E A N D E N G I N E E R I N G M A S S A C H U S E T T S I N S T I T U T E O F T E C H N O L O G Y 3.014 Materials Laboratory Fall 2008 Amorphous Polymers:
More informationvan Quantum tot Molecuul
10 HC10: Molecular and vibrational spectroscopy van Quantum tot Molecuul Dr Juan Rojo VU Amsterdam and Nikhef Theory Group http://www.juanrojo.com/ j.rojo@vu.nl Molecular and Vibrational Spectroscopy Based
More informationarxiv: v1 [condmat.soft] 17 Sep 2016
Polyelectrolyte Polypeptide Scaling Laws Via Mechanical and Dielectric Relaxation Measurements Jorge Monreal University of South Florida arxiv:1609.05358v1 [condmat.soft] 17 Sep 2016 Dated: March 1, 2018
More information10. SPONTANEOUS EMISSION & MULTIPOLE INTERACTIONS
P4533 Fall 1995 (Zorn) Atoms in the Radiation Field, 2 page 10.1 10. SPONTANEOUS EMISSION & MULTIPOLE INTERACTIONS In this chapter we address two of the questions that remain as we build a theoretical
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationLecture 8 Polymers and Gels
Lecture 8 Polymers and Gels Variety of polymeric materials Polymer molecule made by repeating of covalently joint units. Living polymers (not considered in this lecture) longchain objects connected by
More informationAnnouncements. Homework 3 (Klaus Schulten s Lecture): Due Wednesday at noon. Next homework assigned. Due Wednesday March 1.
Announcements Homework 3 (Klaus Schulten s Lecture): Due Wednesday at noon. Next homework assigned. Due Wednesday March 1. No lecture next Monday, Feb. 27 th! (Homework is a bit longer.) Marco will have
More informationPhysics 9e/Cutnell. correlated to the. College Board AP Physics 2 Course Objectives
correlated to the College Board AP Physics 2 Course Objectives Big Idea 1: Objects and systems have properties such as mass and charge. Systems may have internal structure. Enduring Understanding 1.A:
More informationOn a Heuristic Point of View about
On a Heuristic Point of View about the and Conversion of A. EINSTEIN exists an essential formal difference between the theoretical pictures physicists have drawn of gases and other ponderable bodies and
More informationMeasuring the size and shape of macromolecules. Hydrodynamics: study of the objects in water How do the move? Translation Rotation
Measuring the size and shape of macromolecules Hydrodynamics: study of the objects in water How do the move? Translation Rotation 1) Movement with no external forcefree diffusion 2) Movement under the
More informationV. Electrostatics Lecture 24: Diffuse Charge in Electrolytes
V. Electrostatics Lecture 24: Diffuse Charge in Electrolytes MIT Student 1. PoissonNernstPlanck Equations The NernstPlanck Equation is a conservation of mass equation that describes the influence of
More informationInfinite series, improper integrals, and Taylor series
Chapter 2 Infinite series, improper integrals, and Taylor series 2. Introduction to series In studying calculus, we have explored a variety of functions. Among the most basic are polynomials, i.e. functions
More informationTHE NATURE OF THERMODYNAMIC ENTROPY. 1 Introduction. James A. Putnam. 1.1 New Definitions for Mass and Force. Author of
THE NATURE OF THERMODYNAMIC ENTROPY James A. Putnam Author of http://newphysicstheory.com james@newphysicstheory.com Thermodynamic entropy is a pathway for transitioning from the mechanical world of fundamental
More informationMATERIALS SCIENCE POLYMERS
POLYMERS 1) Types of Polymer (a) Plastic Possibly the largest number of different polymeric materials come under the plastic classification. Polyethylene, polypropylene, polyvinyl chloride, polystyrene,
More informationAn electrokinetic LB based model for ion transport and macromolecular electrophoresis
An electrokinetic LB based model for ion transport and macromolecular electrophoresis Raffael Pecoroni Supervisor: Michael Kuron July 8, 2016 1 Introduction & Motivation So far an mesoscopic coarsegrained
More informationAdvanced sampling. fluids of strongly orientationdependent interactions (e.g., dipoles, hydrogen bonds)
Advanced sampling ChE210D Today's lecture: methods for facilitating equilibration and sampling in complex, frustrated, or slowevolving systems Difficulttosimulate systems Practically speaking, one is
More informationElastic Scattering. R = m 1r 1 + m 2 r 2 m 1 + m 2. is the center of mass which is known to move with a constant velocity (see previous lectures):
Elastic Scattering In this section we will consider a problem of scattering of two particles obeying Newtonian mechanics. The problem of scattering can be viewed as a truncated version of dynamic problem
More informationSmall Angle Xray Scattering (SAXS)
Small Angle Xray Scattering (SAXS) We have considered that Bragg's Law, d = λ/(2 sinθ), supports a minimum size of measurement of λ/2 in a diffraction experiment (limiting sphere of inverse space) but
More informationComputer simulation methods (2) Dr. Vania Calandrini
Computer simulation methods (2) Dr. Vania Calandrini in the previous lecture: time average versus ensemble average MC versus MD simulations equipartition theorem (=> computing T) virial theorem (=> computing
More informationBasic Laboratory. Materials Science and Engineering. Atomic Force Microscopy (AFM)
Basic Laboratory Materials Science and Engineering Atomic Force Microscopy (AFM) M108 Stand: 20.10.2015 Aim: Presentation of an application of the AFM for studying surface morphology. Inhalt 1.Introduction...
More informationFinite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras. Module  01 Lecture  11
Finite Element Analysis Prof. Dr. B. N. Rao Department of Civil Engineering Indian Institute of Technology, Madras Module  01 Lecture  11 Last class, what we did is, we looked at a method called superposition
More informationPhysikalisches Praktikum für Fortgeschrittene 1 Dielectric Constant Assistent: Herr Dr. M. Ghatkesar by Therese Challand theres.
Physikalisches Praktikum für Fortgeschrittene 1 Dielectric Constant Assistent: Herr Dr. M. Ghatkesar by Therese Challand theres.challand stud.unibas.ch Contents 1 Theory 1 1.1 Introduction............................
More informationMath Methods for Polymer Physics Lecture 1: Series Representations of Functions
Math Methods for Polymer Physics ecture 1: Series Representations of Functions Series analysis is an essential tool in polymer physics and physical sciences, in general. Though other broadly speaking,
More informationCurvature Distribution of Wormlike Chains in Two and Three Dimensions
Curvature Distribution of Wormlike Chains in Two and Three Dimensions Shay M. Rappaport, Shlomi Medalion and Yitzhak Rabin Department of Physics, BarIlan University, RamatGan 59, Israel arxiv:8.383v
More informationSupporting Information
Supporting Information A: Calculation of radial distribution functions To get an effective propagator in one dimension, we first transform 1) into spherical coordinates: x a = ρ sin θ cos φ, y = ρ sin
More informationCH 24. Electric Potential
CH 24 Electric Potential [SHIVOK SP212] January 8, 2016 I. Electric Potential Energy A. Experimentally, physicists and engineers discovered that the electric force is conservative and thus has an associated
More informationLecture 24 Origins of Magnetization (A number of illustrations in this lecture were generously provided by Prof. Geoffrey Beach)
Lecture 4 Origins of Magnetization (A number of illustrations in this lecture were generously provided by Prof. Geoffrey Beach) Today 1. Magnetic dipoles.. Orbital and spin angular momenta. 3. Noninteracting
More informationAnalysis of NMR Spectra Part 2
Analysis of NMR Spectra Part 21 Analysis of NMR Spectra Part 2 "Things should be made as simple as possible, but not any simpler." Albert Einstein 1.1 Review of Basic NMR Concepts NMR analysis is a complex
More informationIntroduction to polymer physics Lecture 1
Introduction to polymer physics Lecture 1 Boulder Summer School July August 3, 2012 A.Grosberg New York University Lecture 1: Ideal chains Course outline: Ideal chains (Grosberg) Real chains (Rubinstein)
More information31. Diffraction: a few important illustrations
31. Diffraction: a few important illustrations Babinet s Principle Diffraction gratings Xray diffraction: Bragg scattering and crystal structures A lens transforms a Fresnel diffraction problem into a
More informationLab Week 4 Module α 1. Polymer chains as entropy springs: Rubber stretching experiment and XRD study. Instructor: Gretchen DeVries
3.014 Materials Laboratory December 914, 005 Lab Week 4 Module α 1 Polymer chains as entropy springs: Rubber stretching experiment and XRD study Instructor: Gretchen DeVries Objectives Review thermodynamic
More informationChapter 9: Statistical Mechanics
Chapter 9: Statistical Mechanics Chapter 9: Statistical Mechanics...111 9.1 Introduction...111 9.2 Statistical Mechanics...113 9.2.1 The Hamiltonian...113 9.2.2 Phase Space...114 9.2.3 Trajectories and
More informationRENORMALIZATION OF DYSON S VECTORVALUED HIERARCHICAL MODEL AT LOW TEMPERATURES
RENORMALIZATION OF DYSON S VECTORVALUED HIERARCHICAL MODEL AT LOW TEMPERATURES P. M. Bleher (1) and P. Major (2) (1) Keldysh Institute of Applied Mathematics of the Soviet Academy of Sciences Moscow (2)
More informationV(φ) CH 3 CH 2 CH 2 CH 3. High energy states. Low energy states. Views along the C2C3 bond
Example V(φ): Rotational conformations of nbutane C 3 C C C 3 Potential energy of a nbutane molecule as a function of the angle φ of bond rotation. V(φ) Potential energy/kj mol 1 0 15 10 5 eclipse gauche
More informationLongrange manybody polyelectrolyte bridging interactions
THE JOURNAL OF CHEMICAL PHYSICS 122, 204902 2005 Longrange manybody polyelectrolyte bridging interactions Rudi Podgornik a Department of Physics, University of Ljubljana, Jadranska 19, 1000 Ljubljana,
More informationAP PHYSICS 2 FRAMEWORKS
1 AP PHYSICS 2 FRAMEWORKS Big Ideas Essential Knowledge Science Practices Enduring Knowledge Learning Objectives ELECTRIC FORCE, FIELD AND POTENTIAL Static Electricity; Electric Charge and its Conservation
More informationResistance (R) Temperature (T)
CHAPTER 1 Physical Properties of Elements and Semiconductors 1.1 Introduction Semiconductors constitute a large class of substances which have resistivities lying between those of insulators and conductors.
More informationAnirban Som
Anirban Som 011114 Introduction Supramolecular chemistry generates complex structures over a range of length scales. Structures such as DNA origami, supramolecular polymers etc. are formed via multiple
More informationSimulation of CoarseGrained Equilibrium Polymers
Simulation of CoarseGrained Equilibrium Polymers J. P. Wittmer, Institut Charles Sadron, CNRS, Strasbourg, France Collaboration with: M.E. Cates (Edinburgh), P. van der Schoot (Eindhoven) A. Milchev (Sofia),
More informationSelfAssembly. SelfAssembly of Colloids.
SelfAssembly Lecture 56 SelfAssembly of Colloids. Liquid crystallinity Colloidal Stability and Phases The range of forces attractive and repelling forces exists between the colloidal particles van der
More informationInterfacial forces and friction on the nanometer scale: A tutorial
Interfacial forces and friction on the nanometer scale: A tutorial M. Ruths Department of Chemistry University of Massachusetts Lowell Presented at the Nanotribology Tutorial/Panel Session, STLE/ASME International
More informationChapter 2 Kinematical theory of diffraction
Graduate School of Engineering, Nagoya Institute of Technology Crystal Structure Analysis Taashi Ida (Advanced Ceramics Research Center) Updated Oct. 29, 2013 Chapter 2 Kinematical theory of diffraction
More informationGel Permeation Chromatography (GPC) or Size Exclusion Chromatography (SEC)
Gel Permeation Chromatography (GPC) or Size Exclusion Chromatography (SEC) Size Exclusion Chromatography (SEC) is a noninteraction based separation mechanism in which compounds are retained for different
More informationOptical Tweezers. The Useful MicroManipulation Tool in Research
Optical Tweezers The Useful MicroManipulation Tool in Research Student: Nikki Barron Class: Modern Physics/ Biophysics laboratory Advisor: Grant Allen Instructor: David Kleinfeld Date: June 15, 2012 Introduction
More informationLuigi Paolasini
Luigi Paolasini paolasini@esrf.fr LECTURE 5: MAGNETIC STRUCTURES  Mean field theory and magnetic order  Classification of magnetic structures  Collinear and noncollinear magnetic structures.  Magnetic
More informationMechanical Design in Optical Engineering
OPTI Buckling Buckling and Stability: As we learned in the previous lectures, structures may fail in a variety of ways, depending on the materials, load and support conditions. We had two primary concerns:
More informationReview of Strain Energy Methods and Introduction to Stiffness Matrix Methods of Structural Analysis
uke University epartment of Civil and Environmental Engineering CEE 42L. Matrix Structural Analysis Henri P. Gavin Fall, 22 Review of Strain Energy Methods and Introduction to Stiffness Matrix Methods
More informationNuclear magnetic resonance in condensed matter
University of Ljubljana Faculty of mathematics and physics Physics department SEMINAR Nuclear magnetic resonance in condensed matter Author: Miha Bratkovič Mentor: prof. dr. Janez Dolinšek Ljubljana, October
More informationHandout 7 Reciprocal Space
Handout 7 Reciprocal Space Useful concepts for the analysis of diffraction data http://homepages.utoledo.edu/clind/ Concepts versus reality Reflection from lattice planes is just a concept that helps us
More informationFaculty of math and natural science. Universty of Split. KratkyPorod model. Nataša VučemilovidAlagid. February, 2013.
Faculty of math and natural science Universty of Split KratkyPorod model Nataša VučemilovidAlagid February, 2013. Table of contents 1.Introduction:... 3 1. DNA:... 4 2. Models of polymer elasticity:...
More informationThe Principle of Least Action
The Principle of Least Action In their neverending search for general principles, from which various laws of Physics could be derived, physicists, and most notably theoretical physicists, have often made
More informationHydrogels in charged solvents
Hydrogels in charged solvents Peter Košovan, Christian Holm, Tobias Richter 27. May 2013 Institute for Computational Physics Pfaffenwaldring 27 D70569 Stuttgart Germany Tobias Richter (ICP, Stuttgart)
More informationColloid stability. Lyophobic sols. Stabilization of colloids.
Colloid stability. Lyophobic sols. Stabilization of colloids. Lyophilic and lyophobic sols Sols (lyosols) are dispersed colloidal size particles in a liquid medium (=solid/liquid dispersions) These sols
More informationChapter 2 Basis for Indeterminate Structures
Chapter  Basis for the Analysis of Indeterminate Structures.1 Introduction... 3.1.1 Background... 3.1. Basis of Structural Analysis... 4. Small Displacements... 6..1 Introduction... 6.. Derivation...
More informationDeflection of Flexural Members  Macaulay s Method 3rd Year Structural Engineering
Deflection of Flexural Members  Macaulay s Method 3rd Year Structural Engineering 008/9 Dr. Colin Caprani 1 Contents 1. Introduction... 3 1.1 General... 3 1. Background... 4 1.3 Discontinuity Functions...
More informationProblem Set 2 Due Tuesday, September 27, ; p : 0. (b) Construct a representation using five d orbitals that sit on the origin as a basis: 1
Problem Set 2 Due Tuesday, September 27, 211 Problems from Carter: Chapter 2: 2ad,g,h,j 2.6, 2.9; Chapter 3: 1ad,f,g 3.3, 3.6, 3.7 Additional problems: (1) Consider the D 4 point group and use a coordinate
More informationPolymer Physics MSE 458 / CHEM 482 Spring 2017
Polymer Physics MSE 458 / CHEM 482 Spring 2017 Instructor: Prof. A.L. Ferguson 204 MSEB (217) 3002354 alf@illinois.edu Class: Location: 4101 MSEB Time: 2:00 3:20 pm Days: T, Th Sections: A3 (CRN38260)
More informationSOLID STATE PHYSICS. Second Edition. John Wiley & Sons. J. R. Hook H. E. Hall. Department of Physics, University of Manchester
SOLID STATE PHYSICS Second Edition J. R. Hook H. E. Hall Department of Physics, University of Manchester John Wiley & Sons CHICHESTER NEW YORK BRISBANE TORONTO SINGAPORE Contents Flow diagram Inside front
More informationPolymer Physics MSE 458 / CHEM 482 Spring 2018
Polymer Physics MSE 458 / CHEM 482 Spring 2018 Instructor: Prof. A.L. Ferguson 204 MSEB (217) 3002354 alf@illinois.edu Grader: Class: Location: 4101 MSEB Time: 2:00 3:20 pm Days: T, Th Sections: A3 (CRN38260)
More informationarxiv: v1 [physics.classph] 14 Mar 2014
Alberta Thy 514 Current distribution in an infinite plate Andrzej Czarnecki Department of Physics, University of Alberta, Edmonton, Alberta, Canada T6G 2E1 arxiv:1403.3468v1 [physics.classph] 14 Mar
More informationACCURATE FREE VIBRATION ANALYSIS OF POINT SUPPORTED MINDLIN PLATES BY THE SUPERPOSITION METHOD
Journal of Sound and Vibration (1999) 219(2), 265 277 Article No. jsvi.1998.1874, available online at http://www.idealibrary.com.on ACCURATE FREE VIBRATION ANALYSIS OF POINT SUPPORTED MINDLIN PLATES BY
More informationExperimental Determination of Crystal Structure
Experimental Determination of Crystal Structure Branislav K. Nikolić Department of Physics and Astronomy, University of Delaware, U.S.A. PHYS 624: Introduction to Solid State Physics http://www.physics.udel.edu/~bnikolic/teaching/phys624/phys624.html
More information6.2 Entropy. 240 CHAPTER 6 Chemical Reactivity and Mechanisms. PRACTICE the skill. APPLY the skill
240 CAPTER 6 Chemical Reactivity and Mechanisms STEP 2 Determine the appropriate sign for each value from step 1. STEP 3 Add the values for all bonds broken and formed. Now we must decide what sign ( or
More informationIntroduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams.
Outline of Continuous Systems. Introduction to Continuous Systems. Continuous Systems. Strings, Torsional Rods and Beams. Vibrations of Flexible Strings. Torsional Vibration of Rods. BernoulliEuler Beams.
More informationTorsion Spring Oscillator with Dry Friction
Torsion Spring Oscillator with Dry Friction Manual Eugene Butikov Annotation. The manual includes a description of the simulated physical system and a summary of the relevant theoretical material for students
More informationTWO CENTER SHELL MODEL WITH WOODSSAXON POTENTIALS
Romanian Reports in Physics, Vol. 59, No. 2, P. 523 531, 2007 Dedicated to Prof. Dorin N. Poenaru s 70th Anniversary TWO CENTER SHELL MODEL WITH WOODSSAXON POTENTIALS M. MIREA Horia Hulubei National Institute
More informationDilution and polydispersity in branched polymers
Des J. Physique Lett. 45 (1984) L199 L203 ler MARS 1984, L199 Classification Physics Abstracts 36.20E 05.40 82.70G Dilution and polydispersity in branched polymers M. Daoud (*), F. Family (**) and G. Jannink
More informationLecture 11: The Stiffness Method. Introduction
Introduction Although the mathematical formulation of the flexibility and stiffness methods are similar, the physical concepts involved are different. We found that in the flexibility method, the unknowns
More informationMoment of inertia. Contents. 1 Introduction and simple cases. January 15, Introduction. 1.2 Examples
Moment of inertia January 15, 016 A systematic account is given of the concept and the properties of the moment of inertia. Contents 1 Introduction and simple cases 1 1.1 Introduction.............. 1 1.
More informationElectrons & Phonons. Thermal Resistance, Electrical Resistance P = I 2 R T = P R TH V = I R. R = f( T)
lectrons & Phonons Ohm s & Fourier s Laws Mobility & Thermal Conductivity Heat Capacity WiedemannFranz Relationship Size ffects and Breadown of Classical Laws 1 Thermal Resistance, lectrical Resistance
More informationPhysics 6010, Fall 2016 Constraints and Lagrange Multipliers. Relevant Sections in Text:
Physics 6010, Fall 2016 Constraints and Lagrange Multipliers. Relevant Sections in Text: 1.3 1.6 Constraints Often times we consider dynamical systems which are defined using some kind of restrictions
More information4. Circular Dichroism  Spectroscopy
4. Circular Dichroism  Spectroscopy The optical rotatory dispersion (ORD) and the circular dichroism (CD) are special variations of absorption spectroscopy in the UV and VIS region of the spectrum. The
More informationA simple model for blockcopolymer layer morphology formation
A simple model for blockcopolymer layer morphology formation A. J. Wagner and A. Croll, Department of Physics, North Dakota State University, Fargo, ND 58102 Prato Workshop, February 12, 2016 A big thanks
More informationScattering Lecture. February 24, 2014
Scattering Lecture February 24, 2014 Structure Determination by Scattering Waves of radiation scattered by different objects interfere to give rise to an observable pattern! The wavelength needs to close
More informationContents. xiii. Preface v
Contents Preface Chapter 1 Biological Macromolecules 1.1 General PrincipIes 1.1.1 Macrornolecules 1.2 1.1.2 Configuration and Conformation Molecular lnteractions in Macromolecular Structures 1.2.1 Weak
More informationThe Oxford Solid State Basics
The Oxford Solid State Basics Steven H. Simon University of Oxford OXFORD UNIVERSITY PRESS Contents 1 About Condensed Matter Physics 1 1.1 What Is Condensed Matter Physics 1 1.2 Why Do We Study Condensed
More information